Effects of quantum statistics of phonons on the thermal conductivity of silicon and germanium nanoribbons
© Kosevich et al.; licensee Springer. 2013
Received: 24 September 2012
Accepted: 11 December 2012
Published: 3 January 2013
We present molecular dynamics simulation of phonon thermal conductivity of semiconductor nanoribbons with an account for phonon quantum statistics. In our semiquantum molecular dynamics simulation, dynamics of the system is described with the use of classical Newtonian equations of motion where the effect of phonon quantum statistics is introduced through random Langevin-like forces with a specific power spectral density (color noise). The color noise describes interaction of the molecular system with the thermostat. The thermal transport of silicon and germanium nanoribbons with atomically smooth (perfect) and rough (porous) edges are studied. We show that the existence of rough (porous) edges and the quantum statistics of phonon change drastically the low-temperature thermal conductivity of the nanoribbon in comparison with that of the perfect nanoribbon with atomically smooth edges and classical phonon dynamics and statistics. The rough-edge phonon scattering and weak anharmonicity of the considered lattice produce a weakly pronounced maximum of thermal conductivity of the nanoribbon at low temperature.
It has been recently shown that silicon and germanium nanowires can give a figure of merit of over 2 at 800 K due to strong reduction of phonon thermal conductivity in nanowires as compared with their equivalent bulk material, i.e., the reduction is caused not only by the alloy disorder, but also by the decrease of the phonon mean free path by reduced-dimensional effects. The effect of temperature on the thermal conductivity of silicon and germanium may be quite different since the Debye temperature of silicon almost doubles that of germanium. The purpose of the present work is to analyze quantum statistic effects on thermal phonon conductivity in silicon and germanium nanoribbons with the use of the novel semiquantum molecular dynamics simulation.
Molecular dynamics is a method of numerical modeling of molecular systems based on classical Newtonian mechanics. It does not allow for the description of pure quantum effects such as the freezing out of high-frequency oscillations at low temperatures and the related decrease to zero of heat capacity for T→0. On the other hand, because of its complexity, a pure quantum-mechanical description does not allow, in general, the detailed modeling of the dynamics of many-body systems. To overcome these obstacles, different semiclassical methods, which allow to take into account quantum effects, have been proposed[3–9].
The most convenient method for numerical modeling is to use the Langevin equations with color-noise random forces[5, 7]. In this approximation, the dynamics of the system is described with the use of classical Newtonian equations of motion while the quantum effects are introduced through random Langevin-like forces with a specific power spectral density (the color noise), which describes the interaction of the molecular system with the thermostat. Here, we apply such semiquantum approach to the simulation of heat transport in low-dimensional nanostructures such as semiconductor nanoribbons with atomically smooth (perfect) and porous (rough) edges. Our previous analytical studies and molecular dynamics simulations have revealed the dramatic decrease of phonon thermal conductivity in quasi-one-dimensional nanostructures with rough (porous) surface and edge layers.
In the semiquantum molecular dynamics approach, the dynamics of the system is described with the use of the classical Newtonian equations of motion while the effects of phonon quantum statistics are introduced through random Langevin-like forces with a specific power spectral density (the color noise). If the random forces are delta-correlated in a time domain, this corresponds to the white noise with a flat power spectral density. This situation corresponds to high-enough temperatures, when k B T is larger than the quantum of the highest phonon frequency mode in the system,. However, for low-enough temperature,, the stochastic dynamics of the system should be described with the use of random Langevin-like forces with a non-flat power spectral density, which corresponds to the system with color noise. For the generation of color noise with the power spectrum, consistent with the quantum fluctuation-dissipation theorem, we use the method which was developed in. The semiquantum molecular dynamics approach has allowed us to model the transition in the rough-edge nanoribbons from the thermal insulator-like behavior at high temperature, when the thermal conductivity decreases with the conductor length (see), to the ballistic conductor-like behavior at low temperature, when the thermal conductivity increases with the conductor length. Here, we apply the semiquantum molecular dynamics approach for the modeling of temperature dependence of thermal phonon conductivity in silicon and germanium nanoribbons with rough edges. We show that the presence of rough edges significantly decreases the room-temperature thermal conductivity of the nanoribbon and results in the weakly pronounced maximum of thermal conductivity at low temperatures. The latter property is closely related with the absence of (or weak) anharmonicity of the lattice potential and correspondingly weak anharmonic (Umklapp) scattering. In our semiquantum molecular dynamics approach, we make use neither of the quantum corrections to classically predicted thermal conductivity, e.g., discussed in, nor of the values of Umklapp or surface roughness-induced scattering rates, calculated independently from molecular dynamics simulation, e.g., discussed in[13, 14]. To diminish the contact (interface) boundary resistance between the nanoribbon and heat reservoirs, e.g., discussed in, we model the nanoribbon with relatively long parts, immersed in semiquantum heat baths (see also).
Results and discussion
We consider a system which consists of K parallel atomic chains in one plane. To model the diamond-like lattice, we assume that each atom has four nearest neighbors. In this connection, we would like to mention that the considered model cannot be applied directly to the predicted[16–19] and recently grown[20, 21] two-dimensional lattice with graphene-like structure, made from Si or Ge atoms, the silicene. Our main goal is to provide semiquantum modeling of the heat transport and effective ‘isotopic effect’ on phonon heat transport in low-dimensional structures made from Si or Ge atoms, arranged in lattices, which reflect the symmetry of corresponding bulk materials. Since the lattice structure (the number of nearest neighbors) of the considered quasi-two-dimensional nanoribbons reflects the bulk one, our model can also be applied to the quasi-three-dimensional nanowires with bulk-like structure. The isotopic effect on phonon heat transport can be used for the understanding and prediction of the trends in the changes of thermal conductivity in low-dimensional nanostructures caused by the essential change in ion masses accompanied by less strong change in inter-ion force constants.
The Hamiltonian of the system describes the kinetic energy and harmonic interparticle interaction potentials. The characteristic energy of the nearest-neighbor interaction energy E0 can be related with the energy of the LO phonon mode in the semiconductor, which is approximately 15 THz in Si and approximately 9 THz in Ge. The ratio of these maximal frequencies is close to the ratio of the Debye temperatures, T D = 645 K in Si and T D = 374 K in Ge, and to the ratio of the inverse square root of Si and Ge atomic masses, which reflect the approximate isotopic effect in phonon properties of Si and Ge lattices when the materials can be described approximately with the same force constants and different atomic masses (see). The particle mass (M) and lattice constant (a) are determined by the mass and characteristic period of the corresponding bulk semiconductor material, a = 5.43 Å and a = 5.658 Å for Si and Ge, respectively.
Semiquantum molecular dynamics simulations with random Langevin-like forces with a specific power spectral density show that quantum statistics of phonons and porosity of edge layers dramatically change the thermal conductivity of Si and Ge nanoribbons at low and room temperatures in comparison with that of the nanoribbons with perfect edges and classical phonon dynamics and statistics. Phonon scattering by the rough edges and weak anharmonicity of the considered lattice produce weakly pronounced maximum of the thermal conductivity of the nanoribbon at low temperature. The approximate isotopic effect is manifested in the scaling of phonon thermal conductivities of the rough-edge nanoribbons with harmonic lattices at elevated temperature. This effect can be used for the prediction of the trends in the changes of phonon thermal conductivity in low-dimensional nanostructures, which was caused by the essential change in atomic masses accompanied by a less strong change in inter-atomic force constants.
The authors thank the financial support given by the project CSD2010-0044, which belongs to the ‘Consolider Ingenio’ Programme of the Spanish Ministry of Finances and Competitiveness.
- Lee EK, Yin L, Lee Y, Lee JW, Lee SJ, Lee J, Cha SN, Whang D, Hwang GS, Hippalgaonkar K, Majumdar A, Yu C, Choi BL, Kim JM, Kim K: Large thermoelectric figure-of-merits from SiGe nanowires by simultaneously measuring electrical and thermal transport properties. Nano Lett 2918, 12: 2012.Google Scholar
- Savin AV, Kosevich Yu A, Cantarero A: Semiquantum molecular dynamics simulation of thermal properties and heat transport in low-dimensional nanostructures. Phys Rev B 2012, 86: 064305.View ArticleGoogle Scholar
- Wang JS: Quantum thermal transport from classical molecular dynamics. Phys Rev Lett 2007, 99: 160601.View ArticleGoogle Scholar
- Donadio D, Galli G: Thermal conductivity of isolated and interacting carbon nanotubes: comparing results from molecular dynamics and the Boltzmann transport equation. Phys Rev Lett 2007, 99: 255502.View ArticleGoogle Scholar
- Heatwole EM, Prezhdo OV: Second-order Langevin equation in quantized Hamilton dynamics. J Physical Soc Jpn 2008, 77: 044001. 10.1143/JPSJ.77.044001View ArticleGoogle Scholar
- Buyukdagli S, Savin AV, Hu B: Computation of the temperature dependence of the heat capacity of complex molecular systems using random color noise. Phys Rev E 2008, 78: 066702.View ArticleGoogle Scholar
- Ceriotti M, Bussi G, Parrinello M: Nuclear quantum effects in solids using a colored-noise thermostat. Phys Rev Lett 2009, 103: 030603.View ArticleGoogle Scholar
- Dammak H, Chalopin Y, Laroche M, Hayoun M, Greffet JJ: Quantum thermal bath for molecular dynamics simulation. Phys Rev Lett 2009, 103: 190601.View ArticleGoogle Scholar
- Wang JS, Ni X, Jiang JW: Molecular dynamics with quantum heat baths: application to nanoribbons and nanotubes. Phys Rev B 2009, 80: 224302.View ArticleGoogle Scholar
- Kosevich YuA: Multichannel propagation and scattering of phonons and photons in low-dimension nanostructures. Physics-Uspekhi 2008, 51: 848.View ArticleGoogle Scholar
- Kosevich Yu A, Savin AV: Reduction of phonon thermal conductivity in nanowires and nanoribbons with dynamically rough surfaces and edges. Europhys Lett 2009, 88: 14002. 10.1209/0295-5075/88/14002View ArticleGoogle Scholar
- Turney JE, McGaughey AJH, Amon CH: Assessing the applicability of quantum corrections to classical thermal conductivity predictions. Phys Rev B 2009, 79: 224305.View ArticleGoogle Scholar
- Mingo N: Calculation of Si nanowire thermal conductivity using complete phonon dispersion relations. Phys Rev B 2003, 68: 113308.View ArticleGoogle Scholar
- Martin P, Aksamija Z, Pop E, Ravaioli U: Impact of phonon-surface roughness scattering on thermal conductivity of thin Si nanowires. Phys Rev Lett 2009, 102: 125503.View ArticleGoogle Scholar
- Zhang W, Mingo N, Fisher TS: Simulation of phonon transport across a non-polar nanowire junction using an atomistic Green’s function method. Phys Rev B 2007, 76: 195429.View ArticleGoogle Scholar
- Roethlisberger U, Andreoni W, Parrinello M: Structure of nanoscale silicon clusters. Phys Rev Lett 1994, 72: 665. 10.1103/PhysRevLett.72.665View ArticleGoogle Scholar
- Takeda K, Shiraishi K: Theoretical possibility of stage corrugation in Si and Ge analogs of graphite. Phys Rev B 1994, 50: 14916. 10.1103/PhysRevB.50.14916View ArticleGoogle Scholar
- Cahangirov S, Topsakal M, Aktuerk E, Seahin H, Ciraci S: Two- and one-dimensional honeycomb structures of silicon and germanium. Phys Rev Lett 2009, 102: 236804.View ArticleGoogle Scholar
- Houssa M, Pourtois G, Afanasiev VV, Stesmans A: Can silicon behave like graphene? A first-principles study. Appl Phys Lett 2010, 97: 112106. 10.1063/1.3489937View ArticleGoogle Scholar
- Vogt P, De Padova P, Quaresima C, Avila J, Frantzeskakis E, Asensio MC, Resta A, Ealet B, Le Lay G: Silicene: compelling experimental evidence for graphenelike two-dimensional silicon. Phys Rev Lett 2012, 108: 155501.View ArticleGoogle Scholar
- Fleurence A, Friedlein R, Ozaki T, Kawai H, Wang Y, Yamada-Takamura Yu: Experimental evidence for epitaxial silicene on diboride thin films. Phys Rev Lett 2012, 108: 245501.View ArticleGoogle Scholar
- Ziman JM: Electrons and Phonons. Oxford: Oxford University Press; 1960.Google Scholar
- Klitsner T, VanCleve JE, Fisher HE, Pohl RO: Phonon radiative heat transfer and surface scattering. Phys Rev B 1988, 38: 7576. 10.1103/PhysRevB.38.7576View ArticleGoogle Scholar
- Lim J, Hippalgaonkar K, Andrews SC, Majumdar A, Yang P: Quantifying surface roughness effects on phonon transport in silicon nanowires. Nano Lett 2475, 12: 2012.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License(http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.